Synthesis and properties of Fe3O4-activated carbon magnetic nanoparticles for removal of aniline from aqueous solution: equilibrium, kinetic and thermodynamic studies
© Kakavandi et al; licensee BioMed Central Ltd. 2013
Received: 31 July 2012
Accepted: 13 January 2013
Published: 17 February 2013
In this study, powder activated carbon (PAC) and magnetic nanoparticles of iron (III) oxide were used for synthesis of Fe3O4-activated carbon magnetic nanoparticles (AC-Fe3O4 MNPs) as an adsorbent for the removal of aniline. The characteristics of adsorbent were evaluated by SEM, TEM, XRD and BET. Also, the impact of different parameters such as pH, contact time, adsorbent dosage, aniline initials concentration and solution temperature were studied. The experimental data investigated by Langmuir and Freundlich adsorption isotherms and two models kinetically of pseudo first-order and pseudo second-order. The results indicated that the adsorption followed Langmuir and pseudo second-order models with correlation r2 > 0.98 and r2 > 0.99, respectively. The equilibrium time was obtained after 5 h. According to Langmuir model, the maximum adsorption capacity was 90.91 mg/g at pH = 6, and 20°C. The thermodynamic parameters indicated that adsorption of aniline on magnetic activated carbon was exothermic and spontaneous. This synthesized AC-Fe3O4 MNPs due to have advantages such as easy and rapid separation from solution could be applied as an adsorbent effective for removal of pollutants such as aniline from water and wastewater.
Rapid increasing of industries and subsequently increasing the disposal of pollutants especially organic compounds, to the water resources and environment caused serious and adverse environmental impacts. Aniline is a simple matter with aromatic ring that has a benzene ring and a NH2 bond. It’s used as raw material in petrochemical and agrochemical industries, industries of production of pesticides, rubber, plastics, pharmaceuticals and dyestuff, as well as by-product from paper and textile industries [1, 2]. Aniline was dissolved in water as 3.5% and this solubility increases the presence possibility of this pollutant in such sources. This compound is toxic, carcinogenic and mutagenic, and its presence in human blood caused change of hemoglobin to the Methemoglobin and eventually to disease Cyanosis. Also reiterate and lengthy exposures can cause kidney, Liver, bone and neurological marrow disorders and also loss of anemia, appetite, and weight loss. Thus, aniline presence in water resources even at low concentrations is injurious to aquatic organisms and human health [3, 4]. America Environmental Protection Agency (USEPA) and Europe Economic Committee (EEC) have classified aniline as refractory pollutant .
According to the chemical characteristics and environmental impacts of aniline and the inefficiency of conventional treatment methods for the complete removal of it from the aquatic solution, applying of advanced, quick and effective techniques, is essential. Mainly the most common processes for aniline removal consists of oxidation with ozone , adsorption with activated carbon, clays and other adsorbent [7, 8], biodegradation , electrolysis  and ligand exchanger . But the complete removal of aniline and its derivatives with some of this process is difficult or even impossible and in decomposition processes such as biodegradation and electrolysis, very high cost is the limiting factor. The adsorption process by activated carbon rather than other techniques to remove pollutants even at very low concentrations, because of being in sensitive to pollutants and toxic compounds, allowing recovery of both adsorbent and adsorbate and not forming of dangerous material, such as ozone and free radicals, is very efficient [12, 13].
Activated carbon, due to its structure and high surface area, has been proposed as an adsorbent, and a suitable option for the effective removal of organic contaminations (especially hard-biodegradable pollutants) from aquatic environment. But using of it in large scales (in engineering processes) has been limited because of problems such as filtration, dispersion, create turbidity and high cost of its reduction .
Recently, magnetic separation method has been widely used due to low cost, simplicity and being quick in separation and high efficiency. In this regard, different absorbents such as ion exchange resins, zeolites, activated carbon fibers, polymeric adsorbent and waste and even nanoparticles have been magnetized . The prerequisite for magnetic separation is the synthesizing or combining them with nanoparticles (metal oxides). These nanoparticles that are mainly in the form of Fe3O4 MNPs, were separated or removed accompany with the target pollutants from the aquatic environment by a magnet. Furthermore, the presence of magnetic iron oxide (Fe3O4) leads to chemical stability, low toxicity, and excellent recyclability of adsorbent and these have been caused to widely use of this method for removal of toxic ions and organic contaminants from water and wastewater and according to conducted studies these material itself, have high capacity to remove pollutants . In this study new bed has been provided to aniline removal and laboratory conditions have been optimized to increase the absorption capacity. Therefore, the aim of this study was synthesizing magnetic nanoparticles of Fe3O4- activated carbon (AC-Fe3O4 MNPs) as an adsorbent for the adsorption of aniline from synthetic wastewater samples.
Materials and methods
Chemicals and instruments
All the components were analytical reagent-grade and used as supplied. Nitric acid (HNO3 65%), ferric nitrate (Fe (NO3)3.9H2O), powder activated carbon (PAC) and aniline were purchased from Merck. In all of experiments is used double distilled deionized water and pH meter (HACH-HQ-USA) for control pH solution (±0.01) and for determination of aniline residual concentrations applied UV-Visible spectrophotometer (CECIL CE7400). In order to magnetic separation of adsorbent from aqueous solution also used a magnetic field with an intensity of 1.3 T (5 × 5 × 4 cm).
Preparation of activated carbon-Fe3O4 magnetic nanoparticles (AC-Fe3O4MNPs)
The Fe3O4-activated carbon magnetic nanoparticles (AC-Fe3O4 MNPs) were prepared by a chemical co-precipitation method. Synthesis of Fe3O4 nanoparticles and combine it with activated carbon was according to the technique given by Do et al. with small alters . At the first, especially amount of activated carbon was impregnated in the nitric acid (63%) to 3 h in 80°C for make hydrophilic with using an ultrasonic bath. The sample then were filtrated and dried in a room temperature. Subsequently, 5 g of obtained powder impregnated into a 200 mL of aqueous solution containing Fe3O4.9H2O and placed in ultrasonic vibration for a 1 h at 80°C. Then sample was filtrated and dehydrated in an oven at 105°C for 1 h. The samples were heated inside of a furnace in 750°C within 3 h under nitrogen gas in other to formation of AC-Fe3O4 magnetic nanoparticles. Finally, the synthesized adsorbent two washed with deionized water four times and then dried at a 105°C and kept in desiccators for use.
Characterization of the adsorbent
The specific surface area, volume and pore size distributions of AC-Fe3O4 magnetic nanoparticles were measured by Brunner, Emmett and Teller (BET) and Barrett, Joyner and Halenda (BJH)(Quantachrome, NOVA2000) using method of N2 isotherms. In order to determination of composition crystalline structures and X-ray diffraction (XRD) pattern nanoparticles Fe3O4 applied of a powder X-ray diffraction (Quantachrome, NOVA2000) using Cu-kα radiation, λ = 1.54 Å at 25°C. The surface physical morphology, shape and size of Fe3O4 nanoparticle were analyzed using scanning electron microscopy (SEM, PHILIPS, XL-30) and transmission electron microscopy (TEM, PHILIPS, EM 208).
Aniline adsorption optimization
Where C0 and Ce are the initial and equilibrium (final) concentrations of aniline (mg/L) and w is the concentration of AC-Fe3O4 MNPs (g/L).
Adsorption isotherms of aniline
Where q0 (mg/g) is the solid phase equilibrium concentration of aniline, k1 (L/mg) are Langmuir adsorption constant and Ce (mg/L) is the equilibrium concentration of the aniline in the liquid phase. kF (mg/g)(L/mg)1/n ) and n (unitless) are the parameters related to the adsorption capacity and intensity of Freundlich, respectively. The values of n indicate the type of adsorption to be favorable (range of 2–10), moderately difficult (in the range of 1–2) or poor adsorption (n < 1). The fundamental properties of the Langmuir isotherm can be explain in terms of dimensionless separation factor RL:(RL = 1/(1 + kLC0)). The factor of RL indicates the type of the isotherm to be unfavorable (RL > 1), favorable (0 < RL > 1), irreversible (RL = 0) and linear adsorption (RL = 1).
Adsorption kinetics of aniline
Where qe and qt (mg/g) are the amount of aniline adsorbed at equilibrium and at time t (min), respectively. k1 (1/min) and K2 (g/(mg.min)) are rate constants of the first order and second order adsorption, respectively.
Aniline adsorption thermodynamics
Parameters of adsorption equilibrium isotherms for An on AC-Fe 3 O 4 MNPs
Kinetic parameters for adsorption of An on AC-Fe 3 O 4 MNPs
Initial an concentration
Thermodynamic parameters of aniline adsorption on AC-Fe 3 O 4 MNPs
Characterization of the adsorbent
In order to determine crystal phase of iron oxide particles, the sample were analyzed by powder X-ray diffraction (XRD) in the 2θ in region of 10-70o at 25°C by using Cu kα radiation (λ = 1.54Å). Figure 1 shows XRD pattern for the synthesized adsorbent. The highest peaks of AC-Fe3O4 MNPs at 2θ value of 30.2o، 35.5o، 54.9o and 62.9o corresponded to (172), (342), (511), (122) and (106) planes, which by comparison with JCPDS NO. 01-088-0866 was confirmed presence crystals of magnetic nanoparticles Fe3O4 with a cubic structure (2θ = 35.5o). So, this analysis illustrate that Fe3O4 magnetic nanoparticles were on powder activated carbon successfully were synthesized. In previously studies similar this results was reported [18, 19].
The morphology, porosity and texture structure of samples evaluated by using scanning electron microscopy (SEM, Philips XL30) at 25 keV (Figure 2). It can be seen porous with different sizes and shapes and indicated that their distribution on surface of the adsorbent was nearly uniform (Figure 2(a)). Figure 2(b) shows the dispersion of Fe element on activated carbon and so, suggested that nanoparticles iron oxide (Fe3O4) on the adsorbent was alike. In order to investigate size and shape of Fe3O4 nanoparticles, sample was analyzed by using TEM micrographs at 100 keV (Figure 2c), it shows the iron oxide particles with average diameter of 30-80 nm. Figure 2(c) also shows Fe3O4 nanoparticles with a cubic structure which is compatible with results obtained from the analysis of XRD.
Figure 3 shows the N2 adsorption and desorption isotherms, volume and pore size distribution for magnetic nanoparticles of AC-Fe3O4 by applying the methods of BET and BJH at 77.3°K. According to classification of IUPAC, Figure 3(a) exhibit type 4 adsorption isotherms, that reveals the presence of mesopores in adsorbent. Similar results were obtained by another researcher . The results of the BET analysis indicated that the highest surface area of adsorbent was 671.2 m2/g which, in comparison with non-magnetic PAC (1301 m2/g) was reduced . It can be due to presence of Fe3O4 nanoparticles in the structure of activated carbon [16, 21]. Faulconer and et.al reported available surface area decreasing by iron oxides increase, For example at relative of 1:1 C:Fe surface area decreased approximately a 50% . The average pore size measured by BET and BJH was 3.5 and 1.2 nm, respectively which based on IUPAC classification (micropores (d < 2 nm), mesopores (2 < d < 50 nm) and macropores (d > 50 nm)), it (mean size of 3.5 nm) could be classified in mesopores group and the total pore volume by BET obtained 4.87 cc/g at p/p0 = 0.99 and by BJH was 3.7 cc/g (Figure 3(b)).
Optimal conditions for aniline adsorption on magnetic nanoparticles AC- Fe3O4
Optimal pH for uptake of aniline
According to Figure 4(a) in very low pH, electrostatic repulsion between the positive protons of the surface of activated carbon and positive molecules of aniline (or intense competition between H+ and positive charged molecules of aniline) lead to decrease of adsorption capacity. On the other hand, in alkaline pHs, the repulsion of negative charges on the adsorbent and aniline will reduce the adsorption of aniline. The decrease of aniline adsorption under alkaline pH condition may be due to the presence of excess OH- ions and the aniline molecules for the adsorption sites [23, 24]. Zhang and et al. reported the acidic and neutral conditions for favorable removal of aniline using nanoparticles of Fe3O4. Tang et al. reported pH = 6.5 as optimal pH for removal of aniline with granular activated carbon . Therefore pH 6 selected as optimal pH in removing of aniline on magnetic nanoparticles of AC-Fe3O4 and next experiments were conducted in this pH.
Optimal contact time for aniline adsorption
Figure 4(b) reveals that with increase of time from 0 to 400 min was increased the absorbed aniline and it reached to equilibrium in 5 h for the concentrations of 50, 100 and 150 mg/L of aniline and then complete absorption because absorptive capacity remained constant. But in initial concentrations 200 and 300 mg/L the time to reach equilibrium became longer. This may be due to large number of aniline molecules and the dispersion rose from their impact to boundary layer of absorbent. So, the optimal contact time was selected 300 min for absorption of aniline using magnetic nanoparticles. This contact time for removal of aniline by An and et al. reported . Adsorption efficiency at this time for initial concentrations of 50, 100, 150, 200 and 300 mg/L were 80.3, 61.3, 49.9, 42.5 and 40.7%, respectively.
Effect of initial aniline concentration and adsorbent dose
Figure5 demonstrates that by increasing the initial concentration of aniline from 50 mg/L to 300 mg/L in 2 g/L of adsorbent dose, the efficiency decreased from 100 to 58%. The increasing of adsorption efficient in this case may be attributed to the fact that all the adsorbents has a limited number of active sites, which would has become saturated at a specific concentration . However vice versa, adsorption capacity increased with increasing initial aniline concentration. This can be explained that driving forces rising from increasing the aniline concentration . Figure 5 also shows that with increase of adsorbent dose from 0.5 to 2 g/L, in initial concentration of 50 mg/L, enhances the removal efficiency from 37.2 to 100% due to increase sorbent surface or active sites. The increase the in the adsorption efficiency can be due to the increasing availability of aniline molecules to adsorbent surface . The similar results were reported in elimination of aniline with Fe3O4 nanoparticles and activated carbon obtained from oxygen plasma irradiated bamboo [4, 25]. Hence in present study, the amounts of 2 g/L were chosen as optimal adsorbent doses.
Influence of solution temperature on aniline adsorption
As displayed in Figure 6 the results show that with increasing temperature both removal percent and adsorption capacity reduced. Al-Johani et al. (2011) and Tang et al. (2012) in study of aniline removal by carbon nanotube and activated carbon were reported decrease of adsorption efficiency with increasing of temperature [24, 30]. Therefore, decreasing the removal efficiency with increasing temperature indicates that aniline adsorption on AC-Fe3O4 magnetic nanoparticles is exothermic.
It is clear from Table 1 that the correlation coefficient in Longmuir model, for all three investigated temperatures was higher than 0.98. It also observed that the values of RL are between 0 and 1. This shows that the aniline molecules are desirably adsorbed on adsorbent. Thus, according to the regression coefficients obtained from Langmuir and Freundlich models, the adsorption process of aniline follows better from Langmuir model. This suggests that the aniline adsorption on AC-Fe3O4 MNPs was monolayer. Similar results have been reported by Tang et.al (2012) and Wuet.al (2012) in aniline removal using activated carbon [4, 24].
Table 2 shows that the regression coefficients in pseudo second order kinetic model of all initial studied concentrations in compare with the pseudo first order model were higher or almost equal to unit. It also shows that the amounts of calculated capacity (qe,cal) in the pseudo second order model rather than the pseudo first order model were more closer and consistent with adsorption capacity obtained from experiments(qe,exp). According to previous studies, this result suggests that the adsorption behavior of aniline by the studied adsorbent per time unit follows from pseudo second order model and it indicates that the rate-limiting step in aniline adsorption process may be chemisorptions [30, 31].
Aniline adsorption thermodynamic
As shown in Table 3 the values of ΔHo are negative and also ΔGo values for all three temperatures 20, 35 and 50°C were positive. The negative amounts of ΔHo and ΔGo show that the adsorption process of aniline on AC-Fe3O4 MNPs is exothermic and spontaneous. Decreasing of ΔGo with increasing temperature indicates that the adsorption process at higher temperature is undesirable. The negative amounts of ΔSo also indicated that the efficiency is reduced with increasing temperature in solid /liquid phases during adsorption process (or degree of entropy decreases in during the adsorption process). This phenomenon can be resulted from minor changes in the structure of adsorbate and adsorbent at different temperatures.
The magnetic nanoparticles of AC-Fe3O4 with combining iron oxide nanoparticles (IONPs) and powder activated carbon, were successfully synthesized and used in the removal of aniline from aqueous environments. Results revealed that the adsorption efficiency of aniline on this adsorbent was better at pH close to neutral and it was enhanced with increasing the contact time and adsorbent dosage, but reduced with increasing initial aniline concentration and temperature. Equilibrium and kinetic studies indicated that the adsorption was fit with Langmuir and pseudo second order, respectively and thermodynamic studies also showed that the adsorption aniline on AC-Fe3O4 MNPs has been spontaneous and exothermic. The present study showed that nanoparticles of AC-Fe3O4 in addition to having features such as easy separation and extraction solution and need no filtration, have proper porosity, surface area and also good adsorption capacity. This adsorbent can be used as effectively and efficiently adsorbent to remove most contaminants, especially organic pollutants from aquatic environment.
This study was done by financial support of Tehran University of Medical Sciences and Iranian Nano Technology Initiative Council.
- Qi XH, Zhuang YY, Yuan YC, Gu WX: Decomposition of aniline in Supercritical water. J Hazard Mater. 2002, 90 (14): 51-62.View ArticleGoogle Scholar
- Tang HQ, Li J, Bie Y, Zhu L, Zou J: Photochemical removal of aniline in aqueous solutions: switching from photocatalytic degradation to photo-enhanced polymerization recovery. J Hazard Mater. 2010, 175 (1–3): 977-984.View ArticleGoogle Scholar
- Kamble SP, Sawant SB, Schouten JC: Photocatalytic and photochemical degradation of aniline using concentrated solar radiation. J Chem Technol Biotechnol. 2003, 78: 865-872. 10.1002/jctb.867.View ArticleGoogle Scholar
- Guang-Qian W, Zhang X, Hui H: Adsorptive removal of aniline from aqueous solution by oxygen plasma irradiated bamboo based activated carbon. J Chem Eng. 2012, 185–186: 201-210.Google Scholar
- Li JM, Jin ZX: Effect of hypersaline aniline-containing pharmaceutical wastewater on the structure of activated sludge-derived bacterial community. J Hazard Mater. 2009, 172: 432-438. 10.1016/j.jhazmat.2009.07.031.View ArticleGoogle Scholar
- Faria PCC, Órfão JJM, Pereira MFR: Ozonation of aniline promoted by activated carbon. J Chemosphere. 2007, 67: 809-815. 10.1016/j.chemosphere.2006.10.020.View ArticleGoogle Scholar
- Xie X, Gao L, Sun J: Thermodynamic study on aniline adsorption on chemical modified multi-walled carbon nanotubes. J Colloid Surf A. 2007, 308: 54-59. 10.1016/j.colsurfa.2007.05.028.View ArticleGoogle Scholar
- Unuabonah EI, Adebowale KO, Dawodu FA: Equilibrium, kinetic and sorber design studies on the adsorption of aniline blue dye by sodium tetraborate modified kaolinite clay adsorbent. J Hazard Mater. 2008, 157: 397-409. 10.1016/j.jhazmat.2008.01.047.View ArticleGoogle Scholar
- Orshansky F, Narkis N: Characteristics of organics removal by PACT simultaneous adsorption and biodegradation. J Water Res. 1997, 31: 391-398. 10.1016/S0043-1354(96)00227-8.View ArticleGoogle Scholar
- Han Y, Quan X, Chen S, Zhao H: Electrochemically enhanced adsorption of aniline on activated carbon fibers. Sep Purif Technol. 2006, 50: 365-372. 10.1016/j.seppur.2005.12.011.View ArticleGoogle Scholar
- Gürten AA, Uc S, Özler MA: Removal of aniline from aqueous solution by PVC-CDAE ligand-exchanger. J Hazard Mater. 2005, 120: 81-87. 10.1016/j.jhazmat.2004.11.031.View ArticleGoogle Scholar
- Al-Ghouti MA, Li J, Salamh Y: Adsorption mechanisms of removing heavy metals and dyes from aqueous solution using date pits solid adsorbent. J Hazard Mater. 2010, 176: 510-520. 10.1016/j.jhazmat.2009.11.059.View ArticleGoogle Scholar
- Iram M, Guo C, Guan Y: Adsorption and magnetic removal of neutral red dye from aqueous solution using Fe3O4 hollow nanospheres. J Hazard Mater. 2010, 181: 1039-1050. 10.1016/j.jhazmat.2010.05.119.View ArticleGoogle Scholar
- Ai L, Jiang J: Fast removal of organic dyes from aqueous solutions by AC/ferrospinel composite. Desalination. 2010, 262: 134-140. 10.1016/j.desal.2010.05.059.View ArticleGoogle Scholar
- Li Q, Wu S, Liu G, Liao X: Simultaneous biosorption of cadmium(II) and lead (II) ions by pretreated biomass of phane- rochaetechrysosporium. Sep Purif Technol. 2004, 34: 925-940.Google Scholar
- Guo Z, Feng R, Li J: Degradation of 2,4-dinitrophenol by combining sonolysis and different additives. J Hazard Mater. 2008, 158: 164-169. 10.1016/j.jhazmat.2008.01.056.View ArticleGoogle Scholar
- Do MH, Phan NH, Nguyen TD: Activated carbon/Fe3O4 nanoparticle composite: Fabrication, methyl orange removal and regeneration by hydrogen peroxide. Chemosphere. 2011, 85: 1269-1279. 10.1016/j.chemosphere.2011.07.023.View ArticleGoogle Scholar
- Liu Z, Zhang F-S, Sasai R: Arsenate removal from water using Fe3O4 loaded activated carbon prepared from waste biomass. J Chem Eng. 2010, 160: 57-62. 10.1016/j.cej.2010.03.003.View ArticleGoogle Scholar
- Pang Y, Zeng G, Tang Y: Preparation and application of stability enhanced magnetic nanoparticles for rapid removal of Cr(VI). J Chem Eng. 2011, 175: 222-227.View ArticleGoogle Scholar
- Huang L, Sun Y, Wang W: Comparative study on characterization of activated carbons prepared by microwave and conventional heating methods and application in removal of oxytetracycline (OTC). J Chem Eng. 2011, 171: 1446-1453. 10.1016/j.cej.2011.05.041.View ArticleGoogle Scholar
- Mendez-Diaz JD, Prados-Joya G, Rivera-Utilla J: Kinetic study of the adsorption of nitroimidazole antibiotics on activated carbons in aqueous phase. J Colloid Inter Sci. 2010, 345: 481-490. 10.1016/j.jcis.2010.01.089.View ArticleGoogle Scholar
- Faulconer EK, Hoogesteijn von Reitzenstein NV, Mazyck DW: Optimization of magnetic powdered activated carbon for aqueous Hg(II) removal and magnetic recovery. J Hazard Mater. 2011, 199–200: 9-14.Google Scholar
- Zheng H, Liu D, Zheng Y, Liang S, Liu Z: Sorption isotherm and kinetic modeling of aniline on Cr-bentonite. J Hazard Mater. 2009, 167: 141-147. 10.1016/j.jhazmat.2008.12.093.View ArticleGoogle Scholar
- Tang B, Liu Y, Yu P: Study of aniline/ε-caprolactam mixture adsorption from aqueous solution onto granular activated carbon: Kinetics and equilibrium. J Chem Eng. 2012, 187: 69-78.View ArticleGoogle Scholar
- Zhang S, Zhao X, Niu H: Superparamagnetic Fe3O4 nanoparticles as catalysts for the catalytic oxidation of phenolic and aniline compounds. J Hazard Mater. 2009, 167: 560-566. 10.1016/j.jhazmat.2009.01.024.View ArticleGoogle Scholar
- An F, Feng X, Gao B: Adsorption property and mechanism of composite adsorbent PMAA/SiO2 for aniline. J Hazard Mater. 2010, 178: 499-504. 10.1016/j.jhazmat.2010.01.109.View ArticleGoogle Scholar
- Lalhruaitluanga H, Jayaram K, Prasad MNV, Kumar KK: Lead(II) adsorption from aqueous solutions by raw and activated charcoals of Melocanna baccifera Roxburgh (bamboo)—A comparative study. J Hazard Mater. 2010, 175: 311-318. 10.1016/j.jhazmat.2009.10.005.View ArticleGoogle Scholar
- Samarghandi MR, Zarrabi M, NooriSepehr M, Amrane A, Safari GH: Application of acidic treated pumice as an adsorbent for the removal of azo dye from aqueous solutions: kinetic, equilibrium and thermodynamic studies. Iran J Environ Health Sci Eng. 2012, 9 (1): 33-44.View ArticleGoogle Scholar
- Khodabakhshi A, Amin MM, Mozaffari M: Synthesis of magnetite nanoparticles and evaluation of its efficiency for arsenic removal from simulated industrial wastewater. Iran J Environ Health Sci Eng. 2011, 8 (3): 189-200.Google Scholar
- Al-Johani H, Abdel Salam M: Kinetics and thermodynamic study of aniline adsorption by multi-walled carbon nanotubes from aqueous solution. J Colloid Inter Sci. 2011, 360: 760-767. 10.1016/j.jcis.2011.04.097.View ArticleGoogle Scholar
- Valderrama C, I.Barios J, Caetano M: Kinetic evaluation of phenol/aniline mixtures adsorption from aqueous solutions onto activated carbon and hyper cross linked polymeric resin (MN200). React Funct Polym. 2010, 70: 142-150. 10.1016/j.reactfunctpolym.2009.11.003.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.